- Nano Express
- Open Access
Enhanced optical confinement and lasing characteristics of individual urchin-like ZnO microstructures prepared by oxidation of metallic Zn
© Lu et al.; licensee Springer. 2014
- Received: 14 February 2014
- Accepted: 1 April 2014
- Published: 11 April 2014
We prepared urchin-like micron-sized ZnO cavities with high optical quality by oxidizing metallic Zn and proposed the mechanism that resulted in the growth of the urchin-like microstructures. The photoluminescence spectra of the ZnO microstructures had a predominant excitonic emission at room temperature. The lasing properties of the urchin-like ZnO microstructures were investigated systematically through excitation power- and size-dependent photoluminescence measurements. The results showed that a low lasing threshold with high quality factors could be achieved because of the high reflectivity of the optical reflectors formed by the tapered nanowires. The unique optical characteristics may facilitate the development of high-efficiency random lasers.
- Random laser
The miniaturization of light sources is one of the key issues for the development of smaller optoelectronic devices with enhanced functions and properties [1–4]. Zinc oxide (ZnO) materials have attracted increased attention in recent years to realize efficient UV emitters because of their large direct bandgap of 3.37 eV and large free exciton binding energy of 60 meV [5–7]. Remarkable efforts have already been devoted to the synthesis of various ZnO nano/microstructures such as nanowires, nanobelts, nanoribbons, nanorods, and microdisks, which serve as the most promising building blocks for nano/microsized optoelectronic devices [8–16]. UV lasing action at room temperature using ZnO nano/microstructures has significantly spurred the research interest. The lasing characteristics of ZnO micro/nanostructures can generally be classified into two feedback mechanisms: microcavity lasing and random lasing (RL). In the case of microcavity lasing, light confinement is attributed to the high refractive index of ZnO, and the light can be amplified within a single ZnO micro/nanocrystal. There are two ways of confining light: using a Fabry-Pérot (F-P) cavity in a ZnO nanowire [2, 8, 9] and using a whispering-gallery mode (WGM) cavity in a single ZnO microrod [7, 15, 17] or microdisk . Because microcavity lasers have a high spatial coherence, the light that emerges from the laser can be focused on a diffraction-limited spot or propagated over a long distance with minimal divergence. On the other hand, RL is caused by light scattering, and random oscillation routes are created by using numerous ZnO micro/nanocrystals or a ZnO microsized composited random medium [10–12, 19, 20]. The coherence properties of RL have been demonstrated in the literature. According to the photon statistics theory, the photon distribution for a coherent light source obeys a Poisson distribution, and the photon distribution for an incoherent light source follows a Bose-Einstein distribution. The temporal coherence properties of a random laser were investigated by using a Michelson interferometer . Cao et al.  studied the photon statistics of a single-shot random laser mode fit to a Poisson-like distribution upon high-intensity pumping. They also addressed the low spatial coherence of RL emission using double-slit experiments . The RL exhibited a high intensity with low spatial coherence due to the stimulated emission in many different spatial modes. Optoelectronic and medical applications require low spatial coherence such as for high-resolution speckle-free imaging. Therefore, it has been conceptually demonstrated that RL is superior to conventional lasing for speckle-free imaging applications .
The RL-related effects have been demonstrated in different ZnO architectures. Most previous studies on RL with ZnO architectures have been accomplished on ensembles [10–12, 19, 20], meaning the properties of the individual microstructures were missing in the superposition of the ensemble. However, the RL characteristics of single microstructures have not been investigated so far. A detailed investigation on the lasing behaviors of the individual ZnO microstructures is crucial for micro/nanolaser application. In this study, we demonstrated a type of urchin-like ZnO microcrystal formed by oxidizing metallic zinc and revealed the excellent optical quality of these ZnO microstructures. Furthermore, the random lasing behavior of a single urchin-like microstructure was comprehensively examined by employing the excitation power and microstructure size dependence of the photoluminescence emission by pulsed laser excitation.
The synthesis of ZnO microcavities was conducted in two steps. First, hexagonal Zn microcrystals were fabricated using carbothermal vapor-phase transport . This step involved placing a source that contained ZnO powder and graphite powder at a volume ratio of 1:1 into a furnace tube and then placing a Si (100) substrate in a downstream position. After the system was evacuated to a pressure of less than 100 mTorr using a mechanical pump, high-purity argon gas was introduced into the system at a flow rate of 10 sccm. The temperature was kept at 950°C for 1 h, and the pressure in the tube was maintained at 800 mTorr. Then, we conducted an oxidation process. The pressure inside the furnace tube was maintained at 800 mTorr (the same pressure used in the first step) with an O2 flow of 5 sccm, and the oxidation process was conducted at 500°C for 1 h. The synthesized products were characterized by scanning electron microscopy (SEM) and X-ray diffraction (XRD).
For the optical study of a single object, the products were dispersed onto a marked substrate to identify and locate the positions of the individual microcavities. In order to easily locate the excitation area for pumping each individual ZnO microcavity, a 200-mesh transmission electron microscopy grid was fixed on the sample. To measure the photoluminescence, a micro-photoluminescence (μ-PL) system was used to analyze the optical properties of the individual ZnO microcavities under the excitation of a 325-nm HeCd laser or a 266-nm Nd: YAG pulsed laser. The sample was placed on a sample holder that was mounted on a three-axis translational stage. A camera was used to distinguish the signals emitted from individual ZnO microcavities. All of the optical measurements were performed at room temperature.
The growth mechanism of these urchin-like structures was proposed to be self-catalyzed growth resulting from the oxidation of metallic Zn. Figure 2d shows the proposed mechanism by which these urchin-like ZnO microstructures were formed. First, graphite served as a reducing agent. Then, Zn vapor was generated through the carbothermal reduction of ZnO powder at high temperature. The Zn vapor was carried to a low-temperature region by the flow of Ar gas, and the result was the condensation of Zn microcrystals onto the Si substrate located downstream. The zinc microcrystals had the morphology of hexagonally shaped platelets. Second, in the O2 environment that existed during the oxidation process, the as-grown Zn microcrystals were transformed into sheets with side faces that were flat . The oxidation of Zn was caused by the increased surface mobility of the nanosized, liquid Zn droplets and oxygen atoms, which induced the nucleation and growth of ZnO crystals into nanowires. The side face of each flat plane was covered with armlike nanowire structures, hence the name ‘urchin-like’ microstructures.
where R is the reflectivity of the two facets, D is the cavity length, n is the refraction index, and λ is the wavelength. n ~ 2.3 is the refractive index of ZnO, and R = (n − 1)2/(n + 1)2 = 0.16 is the reflectivity at the ZnO/air boundary. When the diameters were 10 and 0.5 μm, the corresponding Q factors were calculated to be 431 and 22, respectively. These values were much smaller than the above Q factor, which indicated that the lasing mechanism was not from the F-P cavity.
In the case of a whispering-gallery mode (WGM), the light was totally reflected by the six lateral sides of the ZnO nanowire at a 60° incident angle because the critical angle of the total internal reflection was approximately 25.8° at the ZnO/air boundary. However, the WGM was difficult to achieve because of the high loss (rough surface) and short gain length in an individual nanowire. Consequently, we excluded that the sharp spectral features were from a few high-quality nanowires.
To confirm the lasing mechanism of the ZnO microcavities, μ-PL measurements of different-sized individual microcavities were made. The PL spectra of different microcavities showed that the spacings between the adjacent sharp peaks were not the same when the sizes and morphologies of the microcavities were different. Therefore, we suggest that the lasing action used should be the RL action . In the urchin-like ZnO microstructures, the body of the microstructures, functioning as an optical gain medium, can provide light amplification. By coherent scattering, the light forms multiple closed-loop optical paths that then serve as laser resonators. The lasing emission wavelength corresponds to the optical path loops in the microstructures. When the amplified light propagates from the body of the microstructure into tapered nanowires, a particular taper diameter is considered as a distributed mirror . The amplified light cannot propagate to the taper, so it returns to the body of the microstructure, which results in efficient optical confinement and the recurrence of the amplified light in the urchin-like microstructure. The laser light eventually escapes through the rough surface of the body.
In order to reveal the light propagation in a ZnO tapered structure, the intensity distributions of electromagnetic fields were simulated using three-dimensional (3D) EigenMode Expansion methods (FIMMPROP), as shown in Figure 4b. Two types of nanotapered nanowires were selected: a highly tapered nanowire and a tapered nanowire with a flat head. We found that a greater fraction of the light was reflected and traveled back to the left inside the nanowire. Interestingly, the fraction of light transmission in the tapered structure with a flat head was greater than that in the highly tapered structure. In other words, the light confinement could be increased in the highly tapered structure. The simulation result indicated that our urchin-like microstructure with multiple-tapered nanowires could improve the light confinement and increase the possibility of light amplification, resulting in a higher Q factor for the urchin-like microstructures compared to other nano/microstructures.
Figure 4c shows the variation in the lasing threshold density as the size of the ZnO microcavities changed. Note that the larger-sized ZnO microcavities had a lower lasing threshold density than the smaller microcavities because the larger volume of the cavities increased the length of the optical gain. Thus, RL could be easily achieved. In addition, the number of resonance modes clearly increased as the size of the cavities increased. The number of lasing modes was also directly related to the size of the microcavities. Figure 4c also shows the number of lasing modes as a function of the size of the microcavities just above their lasing threshold. For the smallest microcavities, only four peaks were observed. As the size of the microcavities increased further, the number of lasing modes increased. The finite size of the cavities limited the number of lasing modes as a result of the gain competition between the random lasing microcavities. If the path loop of the cavity mode spatially overlapped other cavity loops, the lasing behavior did not occur. These results were in agreement with the theoretical calculation for RL .
In conclusion, we reported a simple method for preparing urchin-like ZnO microlaser cavities via the oxidization of metallic Zn. The hexagonal Zn microcrystals were prepared using vapor-phase transport. After the oxidation of the Zn microcrystals, urchin-like ZnO microstructures were formed, and the mechanism of their crystal growth was proposed. For each individual urchin-like ZnO macrostructure, the laser presented a low threshold and high Q factor because the tapered nanowires could serve as effective optical reflectors to improve the optical confinement in the microstructures. The lasing characteristics such as the lasing mode and threshold were investigated. The results are significant for designing architectural nanotapered structures for advanced light management in other optoelectronic devices.
This research is financially supported by the National Science Council of Taiwan under grant NSC-102-2112-M-006-012-MY3 and the Aim for the Top University Project of the Ministry of Education.
- Duan X, Huang Y, Agarwal R, Lieber CM: Single-nanowire electrically driven lasers. Nature 2003, 421: 241–245. 10.1038/nature01353View ArticleGoogle Scholar
- Vanmaekelbergh D, van Vugt LK: ZnO nanowire lasers. Nanoscale 2011, 3: 2783–2800. 10.1039/c1nr00013fView ArticleGoogle Scholar
- Lu YJ, Kim J, Chen HY, Wu C, Dabidian N, Sanders CE, Wang CY, Lu MY, Li BH, Qiu X, Chang WH, Chen LJ, Shvets G, Shih CK, Gwo S: Plasmonic nanolaser using epitaxially grown silver film. Science 2012, 337: 450–453. 10.1126/science.1223504View ArticleGoogle Scholar
- Gu F, Yu H, Fang W, Tong L: Low-threshold supercontinuum generation in semiconductor nanoribbons by continuous-wave pumping. Opt Express 2012, 20: 8667–8674. 10.1364/OE.20.008667View ArticleGoogle Scholar
- Sun HD, Makino T, Tuan NT, Segawa Y, Kawasaki M, Ohtomo A, Tamura K, Koinuma H: Temperature dependence of excitonic absorption spectra in ZnO/Zn0.88 Mg0.12O multiquantum wells grown on lattice-matched substrate. Appl Phys Lett 2001, 78: 2464–2466. 10.1063/1.1367300View ArticleGoogle Scholar
- Okazaki K, Nakamura D, Higashihata M, Iyamperumal P, Okada T: Lasing characteristics of an optically pumped single ZnO nanosheet. Opt Express 2011, 19: 20389–20394. 10.1364/OE.19.020389View ArticleGoogle Scholar
- Trichet A, Sun L, Pavlovic G, Gippius NA, Malpuech G, Xie W, Chen Z, Richard M, Dang LS: One-dimensional ZnO exciton polaritons with negligible thermal broadening at room temperature. Phys Rev B 2011, 83: 041302.View ArticleGoogle Scholar
- Chu S, Wang G, Zhou W, Lin Y, Chernyak L, Zhao J, Kong J, Li L, Ren J, Liu J: Electrically pumped waveguide lasing from ZnO nanowires. Nat Nanotechnol 2011, 6: 506–510. 10.1038/nnano.2011.97View ArticleGoogle Scholar
- Huang MH, Mao S, Feick H, Yan H, Wu Y, Kind H, Weber E, Russo R, Yang P: Room-temperature ultraviolet nanowire nanolasers. Science 2001, 292: 1897–1899. 10.1126/science.1060367View ArticleGoogle Scholar
- Zhu H, Shan CX, Zhang JY, Zhang ZZ, Li BH, Zhao DX, Yao B, Shen DZ, Fan XW, Tang ZK, Hou XH, Choy KL: Low-threshold electrically pumped random lasers. Adv Mater 2010, 22: 1877–1881. 10.1002/adma.200903623View ArticleGoogle Scholar
- Yang HY, Yu SF, Li GP, Wu T: Random lasing action of randomly assembled ZnO nanowires with MgO coating. Opt Express 2010, 18: 13647–13654. 10.1364/OE.18.013647View ArticleGoogle Scholar
- Hsu HC, Wu CY, Cheng HM, Hsieh WF: Band gap engineering and stimulated emission of ZnMgO nanowires. Appl Phys Lett 2006, 89: 013101. 10.1063/1.2218813View ArticleGoogle Scholar
- Hsu HC, Cheng HM, Wu CY, Huang HS, Lee YC, Hsieh WF: Luminescence of selective area growth of epitaxial ZnO nanowires and random-growth-oriented nanobelts. Nanotechnology 2006, 17: 1404–1407. 10.1088/0957-4484/17/5/040View ArticleGoogle Scholar
- Fan HJ, Scholz R, Kolb FM, Zacharias M, Gosele U, Heyroth F, Eisenschmidt C, Hempel T, Christen J: On the growth mechanism and optical properties of ZnO multi-layer nanosheets. Appl Phys A 2004, 79: 1895–1900.View ArticleGoogle Scholar
- Czekalla C, Sturm C, Schmidt-Grund R, Cao BQ, Lorenz M, Grundmann M: Whispering gallery mode lasing in zinc oxide microwire. Appl Phys Lett 2008, 92: 241102. 10.1063/1.2946660View ArticleGoogle Scholar
- Kuo SY, Lin HI: Fabrication and characterization of hexagonally patterned quasi-1D ZnO nanowire arrays. Nanoscale Res Lett 2014, 9: 75. 10.1186/1556-276X-9-75View ArticleGoogle Scholar
- Dai J, Xu CX, Ding R, Zheng K, Shi ZL, Lv CG, Cui YP: Whispering gallery-mode lasing in ZnO microrods at room temperature. Appl Phys Lett 2009, 95: 191117. 10.1063/1.3264080View ArticleGoogle Scholar
- Chen R, Ling B, Sun XW, Sun HD: Room temperature excitonic whispering gallery mode lasing from high-quality hexagonal ZnO microdisks. Adv Mater 2011, 23: 2199–2204. 10.1002/adma.201100423View ArticleGoogle Scholar
- Qiao Q, Shan CX, Zheng J, Zhu H, Yu SF, Li BH, Jia Y, Shen DZ: Surface plasmon enhanced electrically pumped random lasers. Nanoscale 2013, 5: 513–517. 10.1039/c2nr32900jView ArticleGoogle Scholar
- Leong ESP, Yu SF, Lau SP: Directional edge-emitting UV random laser diodes. Appl Phys Lett 2006, 89: 221109. 10.1063/1.2397551View ArticleGoogle Scholar
- Papadakis VM, Stassinopoulos A, Anglos D, Anastasiadis SH, Giannelis EP, Papazoglou DG: Single-shot temporal coherence measurements of random lasing media. J Opt Soc Am B 2007, 24: 31–36. 10.1364/JOSAB.24.000031View ArticleGoogle Scholar
- Cao H, Ling Y, Xu JY, Cao CQ, Kumar P: Photon statistics of random lasers with resonant feedback. Phys Rev Lett 2001, 86: 4524–4527. 10.1103/PhysRevLett.86.4524View ArticleGoogle Scholar
- Redding B, Choma MA, Cao H: Spatial coherence of random laser emission. Opt Lett 2011, 36: 3404–3406. 10.1364/OL.36.003404View ArticleGoogle Scholar
- Redding B, Choma MA, Cao H: Speckle-free laser imaging using random laser illumination. Nat Photonics 2012, 6: 355–359. 10.1038/nphoton.2012.90View ArticleGoogle Scholar
- Leong ESP, Yu SF, Lau SP, Abiyasa AP: Edge-emitting vertically aligned ZnO nanorods random laser on plastic substrate. IEEE Photon Tech Lett 2007, 19: 1792–1794.View ArticleGoogle Scholar
- Tian Y, Ma X, Jin L, Yang D: Electrically pumped ultraviolet random lasing from ZnO films: compensation between optical gain and light scattering. Appl Phys Lett 2010, 97: 251115. 10.1063/1.3531960View ArticleGoogle Scholar
- Cao H, Zhao YG: Random laser action in semiconductor powder. Phys Rev Lett 1999, 82: 2278–2281. 10.1103/PhysRevLett.82.2278View ArticleGoogle Scholar
- Lee SH, Goto T, Miyazaki H, Chang J, Yao T: Optical resonant cavity in a nanotaper. Nano Lett 2010, 10: 2038–2042. 10.1021/nl100100zView ArticleGoogle Scholar
- Ling Y, Cao H, Burin AL, Ratner MA, Liu X, Chang RPH: Investigation of random lasers with resonant feedback. Phys Rev A 2001, 64: 063808.View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/4.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly credited.